In this work, hexavalent chromium adsorption onto LDPE and agave fiber composites coated with chitosan or cellulose was studied in batch experiments. Chemical modifications consisting in cross-linked chitosan, cross-linked chitosan xanthate, and cellulose xanthate were applied to the polysaccharide-coated sorbents in order to increase their stability and adsorption capacity. The sorbents were characterized in terms of morphology by scanning electron microscopy and their chemical composition was evaluated by infrared and nuclear magnetic resonance spectroscopies. The results showed that the adsorption kinetics followed the pseudo-second-order model in all cases (i.e., chemisorption as the rate-limiting step of the adsorption reaction). Moreover, the isotherms evidenced a monolayer adsorption on homogeneous sites described by the Langmuir model. The maximum adsorption capacity of 284.7 mg Cr(VI)/g was obtained for the cross-linked chitosan xanthate sorbent at pH 4 which represents an increase of 43% against the chitosan-coated sorbent (199.1 mg Cr(VI)/g). Besides, functionalized cellulose sorbent also increased its capacity from 84.5 to 106.0 mg Cr(VI)/g cellulose due to the xanthate group. Up to six adsorption-desorption cycles were completed for the case of functionalized chitosan sorbent, confirming that the stability was increased with the cross-linking and the material could be reused several times without losing its adsorption capacity. In the case of cellulose xanthate, only three adsorption cycles were completed. However, improvements were observed in the desorption capacity considering that it decreased below 20% after two cycles in the cellulose-coated sorbent.
This is a preview of subscription content, log in to check access.
Buy single article
Instant unlimited access to the full article PDF.
Price includes VAT for USA
Subscribe to journal
Immediate online access to all issues from 2019. Subscription will auto renew annually.
This is the net price. Taxes to be calculated in checkout.
Afroze, S., & Sen, T. K. (2018). A review on heavy metal ions and dye adsorption from water by agricultural solid waste adsorbents. Water, Air & Soil Pollution, 229(225), 1–50.
Babel, S., & Kurniawan, T. A. (2004). Cr (VI) removal from synthetic wastewater using coconut shell charcoal and commercial activated carbon modified with oxidizing agents and/or chitosan. Chemosphere, 54(7), 951–967.
Boddu, V. M., Abburi, K., Talbott, J. L., & Smith, E. D. (2003). Removal of hexavalent chromium from wastewater using a new composite chitosan biosorbent. Environmental Science & Technology, 37(19), 4449–4456.
Brugnerotto, J., Lizardi, J., Goycoolea, F. M., Argüelles-Monal, W., Desbrieres, J., & Rinaudo, M. (2001). An infrared investigation in relation with chitin and chitosan characterization. Polymer, 42(8), 3569–3580.
Caner, N., Sarı, A., & Tüzen, M. (2015). Adsorption characteristics of mercury (II) ions from aqueous solution onto chitosan-coated diatomite. Industrial & Engineering Chemistry Research, 54(30), 7524–7533.
Dambies, L., Guimon, C., Yiacoumi, S., & Guibal, E. (2001). Characterization of metal ion interactions with chitosan by X-ray photoelectron spectroscopy. Colloids and Surfaces A: Physicochemical and Engineering Aspects, 177, 203–214.
Debnath, S., Maity, A., & Pillay, K. (2014). Magnetic chitosan–GO nanocomposite: Synthesis, characterization and batch adsorber design for Cr (VI) removal. Journal of Environmental Chemical Engineering, 2(2), 963–973.
Deng, Y., Kano, N., & Imaizumi, H. (2017). Adsorption of Cr(VI) onto hybrid membrane of carboxymethyl chitosan and silicon dioxide. Journal of Chemistry, 2017(3426923), 1–8.
El-Reash, Y. G., Otto, M., Kenawy, I. M., & Ouf, A. M. (2011). Adsorption of Cr(VI) and as(V) ions by modified magnetic chitosan chelating resin. International Journal of Biological Macromolecules, 49(4), 513–522.
Elwakeel, K. Z. (2010). Removal of Cr (VI) from alkaline aqueous solutions using chemically modified magnetic chitosan resins. Desalination, 250(1), 105–112.
Fernández-Pazos, M. T., Garrido-Rodriguez, B., Nóvoa-Muñoz, J. C., Arias-Estévez, M., Fernández-Sanjurjo, M. J., Núñez-Delgado, A., et al. (2013). Cr(VI) adsorption and desorption on soils and biosorbents. Water, Air & Soil Pollution, 224, 1366, 1–1366,12.
García-Sánchez, M. E., Pérez-Fonseca, A. A., Gómez, C., González-Reynoso, O., Vázquez-Lepe, M. O., González-Núñez, R., et al. (2017). Improvement of Pb (II) adsorption capacity by controlled alkali treatment to chitosan supported onto agave fiber-HDPE composites. Macromolecular Symposia, 374(1), 1600104.
Habiba, U., Afifi, A. M., Salleh, A., & Ang, B. C. (2017). Chitosan/(polyvinyl alcohol)/zeolite electrospun composite nanofibrous membrane for adsorption of Cr6+, Fe3+ and Ni2+. Journal of Hazardous Materials, 322, 182–194.
Heidari, A., Younesi, H., Mehraban, Z., & Heikkinen, H. (2013). Selective adsorption of Pb (II), Cd (II), and Ni (II) ions from aqueous solution using chitosan–MAA nanoparticles. International Journal of Biological Macromolecules, 61, 251–263.
Hirano, S., Usutani, A., & Midorikawa, T. (1997). Novel fibers of N-acylchitosan and its cellulose composite prepared by spinning their aqueous xanthate solutions. Carbohydrate Polymers, 33(1), 1–4.
Huang, G., Zhang, H., Shi, J. X., & Langrish, T. A. (2009). Adsorption of chromium (VI) from aqueous solutions using cross-linked magnetic chitosan beads. Industrial & Engineering Chemistry Research, 48(5), 2646–2651.
Kalantari, K., Ahmad, M. B., Masoumi, H. R. F., Shameli, K., Basri, M., & Khandanlou, R. (2015). Rapid and high capacity adsorption of heavy metals by Fe3O4/montmorillonite nanocomposite using response surface methodology: Preparation, characterization, optimization, equilibrium isotherms, and adsorption kinetics study. Journal of the Taiwan Institute of Chemical Engineers, 49(4), 192–198.
Kasaai, M. R. (2010). Determination of the degree of N-acetylation for chitin and chitosan by various NMR spectroscopy techniques: a review. Carbohydrate Polymers, 79(4), 801–810.
Kavaklı, C., Barsbay, M., Tilki, S., Güven, O., & Kavaklı, P. A. (2016). Activation of polyethylene/polypropylene nonwoven fabric by radiation-induced grafting for the removal of Cr(VI) from aqueous solutions. Water, Air & Soil Pollution, 227, 473, 1–473,16.
Klapiszewski, Ł., Bartczak, P., Wysokowski, M., Jankowska, M., Kabat, K., & Jesionowski, T. (2015). Silica conjugated with Kraft lignin and its use as a novel ‘green’ sorbent for hazardous metal ions removal. Chemical Engineering Journal, 260, 684–693.
Kulkarni, P. S., Deshmukh, P. G., Jakhade, A. P., Kulkarni, S. D., & Chikate, R. C. (2017). 1,5 diphenylcarbazide immobilized cross-linked chitosan films: an integrated approach towards enhanced removal of Cr (VI). Journal of Molecular Liquids, 247, 254–261.
Kumar, A. S. K., Gupta, T., Kakan, S. S., Kalidhasan, S., Rajesh, V., & Rajesh, N. (2012). Effective adsorption of hexavalent chromium through a three center (3c) co-operative interaction with an ionic liquid and biopolymer. Journal of Hazardous Materials, 239-240, 213–224.
Lin, H., Han, S., Dong, Y., Ling, W., & He, Y. (2018). Structural characteristics and functional properties of corncob modified by hyperbranched polyamide for the adsorption of Cr (VI). Water, Air & Soil Pollution, 229, 117, 1–117,12.
McCormick, C. L., Callais, P. A., & Hutchinson, B. H., Jr. (1985). Solution studies of cellulose in lithium chloride and N, N-dimethylacetamide. Macromolecules, 18(12), 2394–2401.
Mirabedini, M., Kassaee, M. Z., & Poorsadeghi, S. (2017). Novel magnetic chitosan hydrogel film, cross-linked with glyoxal as an efficient adsorbent for removal of toxic Cr(VI) from water. Arabian Journal for Science and Engineering, 45(1), 115–124.
Miretzky, P., & Cirelli, A. F. (2010). Cr (VI) and Cr (III) removal from aqueous solution by raw and modified lignocellulosic materials: a review. Journal of Hazardous Materials, 180(1–3), 1–19.
Ngah, W. W., Ab Ghani, S., & Kamari, A. (2005). Adsorption behaviour of Fe (II) and Fe (III) ions in aqueous solution on chitosan and cross-linked chitosan beads. Bioresource Technology, 96(4), 443–450.
Nguyen, T. C., Loganathan, P., Nguyen, T. V., Vigneswaran, S., Kandasamy, J., & Naidu, R. (2015). Simultaneous adsorption of Cd, Cr, Cu, Pb, and Zn by an iron-coated Australian zeolite in batch and fixed-bed column studies. Chemical Engineering Journal, 270, 393–404.
Pang, L. J., Li, R., Gao, Q. H., Hu, J. T., Xing, Z., Zhang, M. X., et al. (2016). Functionalized and reusable polyethylene fibres for Au (III) extraction from aqueous solution with high adsorption capacity and selectivity. RSC Advances, 6, 87221–87229.
Park, D., Lim, S. R., Yun, Y. S., & Park, J. M. (2008). Development of a new Cr (VI)-biosorbent from agricultural biowaste. Bioresource Technology, 99(18), 8810–8818.
Pérez-Fonseca, A. A., Gómez, C., Dávila, H., González-Núnez, R., Robledo-Ortíz, J. R., Vázquez-Lepe, M. O., et al. (2011). Chitosan supported onto agave fiber—postconsumer HDPE composites for Cr (VI) adsorption. Industrial & Engineering Chemistry Research, 51(17), 5939–5946.
Putro, J. N., Santoso, S. P., Ismadji, S., & Ju, Y. H. (2017). Investigation of heavy metal adsorption in binary system by nanocrystalline cellulose–bentonite nanocomposite: improvement on extended. Langmuir isotherm model. Microporous and Mesoporous Materials, 246(7), 166–177.
Rojas, G., Silva, J., Flores, J. A., Rodriguez, A., Ly, M., & Maldonado, H. (2005). Adsorption of chromium onto cross-linked chitosan. Separation and Purification Technology, 44(1), 31–36.
Sağ, Y., & Aktay, Y. (2002). Kinetic studies on sorption of Cr (VI) and Cu (II) ions by chitin, chitosan and Rhizopus arrhizus. Biochemical Engineering Journal, 12(2), 143–153.
Saleh, T. A. (2015). Isotherm, kinetic, and thermodynamic studies on Hg (II) adsorption from aqueous solution by silica-multiwall carbon nanotubes. Environmental Science and Pollution Research, 22(21), 16721–16731.
Sankararamakrishnan, N., Dixit, A., Iyengar, L., & Sanghi, R. (2006). Removal of hexavalent chromium using a novel cross linked xanthated chitosan. Bioresource Technology, 97(18), 2377–2382.
Schmuhl, R., Krieg, H. M., & Keizer, K. (2001). Adsorption of cu (II) and Cr (VI) ions by chitosan: Kinetics and equilibrium studies. Water SA, 27(1), 1–7.
Soltani, R. D. C., Khorramabadi, G. S., Khataee, A. R., & Jorfi, S. (2014). Silica nanopowders/alginate composite for adsorption of lead (II) ions in aqueous solutions. Journal of the Taiwan Institute of Chemical Engineers, 45(3), 973–980.
Spinelli, V. A., Laranjeira, M. C., & Fávere, V. T. (2004). Preparation and characterization of quaternary chitosan salt: adsorption equilibrium of chromium (VI) ion. Reactive and Functional Polymers, 61(3), 347–352.
Sun, X., Yang, L., Li, Q., Zhao, J., Li, X., Wang, X., et al. (2014). Amino-functionalized magnetic cellulose nanocomposite as adsorbent for removal of Cr (VI): synthesis and adsorption studies. Chemical Engineering Journal, 241, 175–183.
Tingaut, P., Hauert, R., & Zimmermann, T. (2011). Highly efficient and straightforward functionalization of cellulose films with thiol-ene click chemistry. Journal of Materials Chemistry, 21(40), 16066–16076.
Unuabonah, E. I., Olu-Owolabi, B. I., & Adebowale, K. O. (2016). Competitive adsorption of metal ions onto goethite–humic acid-modified kaolinite clay. International journal of Environmental Science and Technology, 13(4), 1043–1054.
Weber, W. J., & Morris, J. C. (1963). Kinetics of adsorption on carbon from solution. Journal of the Sanitary Engineering Division, 89(2), 31–60.
Wu, Z., Li, S., Wan, J., & Wang, Y. (2012). Cr (VI) adsorption on an improved synthesized cross-linked chitosan resin. Journal of Molecular Liquids., 170, 25–29.
Xu, X., Gao, B. Y., Tang, X., Yue, Q. Y., Zhong, Q. Q., & Li, Q. (2011). Characteristics of cellulosic amine-crosslinked copolymer and its sorption properties for Cr (VI) from aqueous solutions. Journal of Hazardous Materials, 189(1), 420–426.
Yakout, A. A., El-Sokkary, R. H., Shreadah, M. A., & Hamid, O. G. A. (2016). Removal of Cd (II) and Pb (II) from wastewater by using triethylenetetramine functionalized grafted cellulose acetate-manganese dioxide composite. Carbohydrate Polymers, 148, 406–414.
Yang, R., Aubrecht, K. B., Ma, H., Wang, R., Grubbs, R. B., Hsiao, B. S., et al. (2015). Thiol-modified cellulose nanofibrous composite membranes for chromium (VI) and lead (II) adsorption. Polymer, 55(5), 1167–1176.
Yu, J. X., Wang, L. Y., Chi, R. A., Zhang, Y. F., Xu, Z. G., & Guo, J. (2015). Adsorption of Pb 2+, Cd 2+, Cu 2+, and Zn 2+ from aqueous solution by modified sugarcane bagasse. Research on Chemical Intermediates, 41(3), 1525–1541.
Zhang, L., Xia, W., Liu, X., & Zhang, W. (2015). Synthesis of titanium cross-linked chitosan composite for efficient adsorption and detoxification of hexavalent chromium from water. Journal of Materials Chemistry A, 3, 331–340.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Moreno-López, A.Y., González-López, M.E., Manríquez-González, R. et al. Evaluation of the Cr(VI) Adsorption Performance of Xanthate Polysaccharides Supported onto Agave Fiber-LDPE Foamed Composites. Water Air Soil Pollut 230, 133 (2019) doi:10.1007/s11270-019-4181-2
- Chitosan xanthate
- Cellulose xanthate